Tensile Testing Laboratory


 Garry Green
 2 years ago
 Views:
Transcription
1 Tensile Testing Laboratory By Stephan Favilla ME 354 AC Date of Lab Report Submission: February 11 th 2010 Date of Lab Exercise: January 28 th
2 Executive Summary Tensile tests are fundamental for understanding properties of different materials, and how they will behave under load. This lab tested four different materials, including A36 hot rolled steel, 6061T6 Aluminum, polycarbonate, and polymethylmethacrylate (PMMA). Each material was tested three times using an Instron load frame and the BlueHill data acquisition software. The data from each test was used to determine valuable material properties such as ultimate tensile strength, modulus of elasticity, and yield strength. Other calculated properties included true fracture strength, percent reduction of area, and percent elongation. These material properties were used for comparing the materials to each other, and to define the material as brittle or ductile. The true stress and true strain were calculated for one sample of 6061T6 aluminum to show the difference between the engineering stress and strain, and the true values. The engineering stress is an assumption that uses the initial area of the cross section, ignoring the effects of transverse strain and the changing cross section. This assumption results in the drop of the engineering stressstrain curve after the ultimate tensile strength, where necking occurs. Using the values of the true strain, the true plastic strain was determined for one sample of Aluminum (Sample #2) by subtracting the contribution of the true elastic strain, as outlined in Appendix E. Plotting the logarithm of the true stress versus the logarithm of the true plastic strain allowed the plastic portion of the true stressstrain curve to be modeled by the RambergOsgood model, as detailed in Appendix F. While the model did poorly at low plastic strains near yielding, it did an excellent job just before necking and the ultimate tensile strain. The results of the tensile tests showed that the A36 hot rolled steel was the strongest material. It had the highest ultimate tensile strength (527.9 MPa), the greatest modulus of toughness (174.6 MPa), and the largest true fracture strength (1047 MPa). The 6061T6 aluminum had a higher yield (356.3 MPa) than the steel (355.6), but a lower ultimate tensile strength (374.9 MPa) and true fracture strength (571.8 MPa) due to tempering and precipitation hardening. All of the materials besides the PMMA proved to be ductile, especially the polycarbonate, which had a percent elongation of 82.2% The PMMA samples averaged a percent elongation of only %. 2
3 A. Introduction Tensile testing is one of the most fundamental tests for engineering, and provides valuable information about a material and its associated properties. These properties can be used for design and analysis of engineering structures, and for developing new materials that better suit a specified use. The tensile testing laboratory was conducted using an Instron load frame and the BlueHill data acquisition software. Four different materials were tested, including 6061T6 Aluminum Alloy, A36 hot rolled steel, polymethylmethacrylate (PMMA, cast acrylic), and polycarbonate. The samples were cylindrical in cross section, with a reduced gage section. The reduced gage section ensured that the highest stresses occurred within the gage, and not near the grips of the Instron load frame, preventing strain and fracture of the specimen near or in the grips. The reduced gage section of each specimen was about 12.7 mm (0.5 inches). The samples were already machined to the proper dimensions required for the test, according to ASTM standards. Three samples of each material were tested in the Instron load frame, and the data gathered into an Excel spreadsheet. The data was used to calculate various properties of each material, including the elastic modulus, yield strength, ultimate tensile strength. The data was then plotted on engineering stressstrain curves to compare the samples. The purpose of this experiment was to gather information about each material so that important mechanical properties could be determined. This experiment also familiarized the students with the Instron load frame, BlueHill data acquisition software, and the general steps to performing a tensile test on a reduced gage section specimen. The data used for this lab report was not gathered from the student run experiments, but rather from standardized testing performed by the laboratory professor, to ensure accurate and consistent results. 3
4 B. Procedure Each specimen was measured with the calipers to determine the diameter of the cross section. A gage length was determined (typically mm) and scribed into the specimen so that the distance between the two marks could be measured after the tensile test was completed. A typical reduced gage section specimen is shown in Figure 1, on the following page. The BlueHill data acquisition software was started, and the correct material was chosen. The load cell was zeroed to ensure that the software only measured the tensile load applied to the specimen. The specimen was loaded into the jaws of the Instron load frame so that it was equally spaced between the two clamps. The axial and transverse extensometers were attached to the reduced gage section of the specimen, ensuring that the axial extensometer was set correctly when attaching it to the gage and that the transverse extensometer was across the complete diameter of the specimen. This precaution results in better data and prevents damage to the extensometers. The Instron load frame, shown in Figure 2 on the following page, was preloaded using the scroll wheel to ensure that the specimen was properly loaded in the frame, and that it wasn t slipping in the jaws. The load was released, and the extensometers were zeroed using the software. The test was started, and the specimen was loaded, resulting in a measureable strain. For the steel and aluminum samples, the crosshead was initially set to move upward at 1.27 mm/min, then at 15 mm/min at a specified state beyond yielding. This increase in the rate of strain sped up the test, but may have also introduced some error. The polycarbonate sample started at 5 mm/min and was later sped up to 30 mm/min. The PMMA samples were pulled at a constant rate of 10 mm/min. The data was gathered using the software, and loaded into a spreadsheet. At a set value of strain (past the yield strain), the software stopped using data from the extensometers, and started gathering the strain information using the position of the moving crosshead. A warning message came up on the computer screen, instructing the operator to remove the 4
5 extensometers to prevent damage. The test continued until fracture, where the software stopped the moving crosshead, and finished gathering data. The specimen was removed, and the crosshead was reset to the initial position to start another tensile test. The testing procedure was repeated for the rest of the specimens. Figure 1: A reduced gage section specimen made from 6061T6 aluminum, ready for tensile testing. Figure 2: A typical Instron load frame used for tensile testing. 5
6 Stress (MPa) Stress (MPa) C. Results C.1 Engineering Stress and Engineering Strain The data from the tensile tests was plotted on separate graphs according to material. Each graph shows the engineering stress versus the engineering strain, as calculated per Appendix A. Figure 3 shows the three tests for the A36 hot rolled steel samples, and Figure 4 shows the three tensile tests of the 6061T6 aluminum samples. Figure 5 and Figure 6 show the test results of the polycarbonate and the PMMA, respectively Steel 1 Steel 2 Steel Strain (m/m) Figure 3: The engineering stress versus the engineering strain for A36 steel Aluminum 1 Aluminum 2 Aluminum Strain (m/m) Figure 4: The engineering stress versus the engineering strain for 6061T6 aluminum. 6
7 Stress (MPa) Stress (MPa) Polycarbonate 1 Polycarbonate 2 Polycarbonate Strain (m/m) Figure 5: The engineering stress versus the engineering strain for polycarbonate PMMA 1 PMMA 2 PMMA Strain (m/m) Figure 6: The engineering stress versus the engineering strain for PMMA. 7
8 C.2 Material Properties The ultimate tensile strength for each material is listed in Table 1. The value of the ultimate tensile strength was found using the process in Appendix B. The strain corresponding to the ultimate tensile strength is where necking begins to occur. Table 1: The ultimate tensile strength for the four materials. Sample Ultimate Tensile Standard Deviation, Material Strength, (MPa) StDev (MPa) A36 Steel T Polycarbonate PMMA The modulus of elasticity and the yield strengths were calculated for steel and aluminum. The corresponding standard deviations for both values were also calculated using the procedure outlined in Appendix B. All of these values are shown in Table 2. Table 2: The modulus of elasticity, yield strength, and standard deviations for steel and aluminum. Modulus of Standard Standard Sample Elasticity, Deviation Yield Strength, Deviation Material E (MPa) of E (MPa) (MPa) of (MPa) A36 Steel T The modulus of resilience and the modulus of toughness were calculated from the area under the engineering stress versus engineering strain curves, as outlined in Appendix C. Both are useful for determining the amount of energy the material can absorb before yielding and fracture. The values of both are shown in Table 3. Table 3: The modulus of resilience and the modulus of toughness for the materials. Sample Material Modulus of Resilience (MPa) Modulus of Toughness (MPa) A36 Steel T Polycarbonate PMMA
9 The true fracture strength provides the actual value of the stress encountered by the sample during the tensile test, just before fracture. The true fracture strength is the greatest stress that the material can handle after yielding. The percent elongation and the percent reduction in area provide information about the ductility of a material, and how much it can be stretched before failure. The calculations of these properties are outlined in Appendix D. The averages of all three values for each of the four materials are shown in Table 4. Table 4: The average true fracture strength, percent reduction of area, and the percent elongation for all four materials. Sample True Fracture Percent Reduction of Percent Elongation, Material Strength, (MPa) Area, %RA %EL A36 Steel % 33.47% 6061T % 17.30% Polycarbonate % 82.20% PMMA % % C.3 True Stress and True Strain One sample of aluminum was used to find the true stress and the true strain encountered during a tensile test, and to compare both to the engineering stress and the engineering strain. The engineering stress and strain does not account for the change in cross sectional area, and only accounts for the axial strain in the sample. The true stress and strain account for the change in cross sectional area, and therefore the true stress is higher than the engineering stress. The true strain is also greater than the engineering strain due to strains in the transverse direction along the gage of the sample. Figure 7 shows the true stress versus the true strain, along with the engineering stress and the engineering strain for the same sample. The second sample of aluminum was used in this analysis, as defined by Appendix E. 9
10 Stress (MPa) True Stress and Strain Engineering Stress and Strain Strain (m/m) Figure 7: The True Stress versus the True Strain, along with the Engineering Stress and Strain for a sample of 6061T6 Aluminum. The true stress at the point of maximum load (where the ultimate tensile strength occurs) for the 6061T6 aluminum sample had a value of MPa, compared to a maximum tensile strength of MPa. The true strain at this point had a value of m/m, compared to an engineering strain of m/m. The maximum true stress at fracture was MPa, with a strain of m/m. At fracture, the engineering stress was MPa, with a strain of m/m. 10
11 True Stress (MPa) C.4 The RambergOsgood Model The behavior of the true stress due to the true plastic strain can be accurately modeled using the RambergOsgood equation. This equation models the stressstrain curve as a power hardening model, after yielding. The resulting equation, as derived in Appendix F, gives rise to Figure 8, where it is plotted against the true stress and strain values derived from the experiment True Plastic Strain (m/m) Calculated Experimental Figure 8: The plot of the true stress versus the true plastic strain for both the experimental values and the calculated values obtained from the RambergOsgood model. The value of the true stress and strain obtained from the RambergOsgood model at three defined points is compared against the experimental values in Table 5, showing the increasing accuracy of the model as plastic strain increases. Table 5: The true stresses calculated using the RambergOsgood model, compared to the experimental true stress. True Plastic Strain (m/m) Calculated Stress (MPa) Experimental Stress (MPa) Percent Error % % % 11
12 D. Discussion The test results were consistent for each of the materials, as evident in Figures 36, where each of the three stressstrain curves were approximately overlapping. An interesting observation can be made from the PMMA graph, where sample one suddenly loses stress as it is stretched. This sample may have fractured partially across the cross section before complete failure, or a void could have caused a sudden release of stress. All of the other samples exhibited consistent behavior. From the ultimate tensile strength data in Table 1, it is clear that the A36 hot rolled steel was the strongest material, followed by aluminum, PMMA, and polycarbonate, respectively. All of the standard deviations were low, not exceeding MPa, suggesting that the data was consistent and that the testing procedure was valid and repeatable. The true fracture strength, shown in Table 4, gives a better view of the true stress at fracture. The A36 steel had the highest true fracture strength, followed by the aluminum, polycarbonate, and PMMA. Although the A36 hot rolled steel had a much higher modulus of elasticity ( MPa, compared to 69460MPa for the 6061T6 aluminum), and a higher ultimate tensile strength, the yield strength is about the same as the 6061T6. The higher ultimate stress is due to work hardening as the material is plastically deformed. The introduction of dislocations reduces their motion, and hardens the material. The 6061T6 is a tempered and aged alloy that is already precipitation hardened. It will not work harden as much as the A36 steel, resulting in a lower ultimate tensile strength. The standard deviations for the yield strength and modulus of elasticity are also small compared to the average values, proving the consistency of the data. The modulus of resilience and the modulus of toughness are important values in determining the energy that a material can absorb before yielding and before fracture. The modulus of resilience is the area under the engineering stressstrain curve up until the yield, and corresponds to the energy per unit volume that a material can absorb before it yields. The 6061T6 aluminum had the highest modulus of resilience, followed by A36 12
13 steel, polycarbonate, and PMMA. The aluminum had the highest resilience due to the high yield strength, and the low modulus of elasticity (compared to the A36 steel), as shown in Table 3. The low modulus of elasticity ensured that the aluminum was strained more before yielding, allowing it to absorb more energy. The modulus of toughness was the highest for the A36 steel due to the high ultimate tensile strength, and the ductility of the steel. The polycarbonate had a higher modulus of toughness than the 6061T6 aluminum due to its high ductility, even though it had a lower yield and ultimate tensile strength. The acrylic had the lowest modulus of toughness due to its brittle nature. The percent reduction of area and the percent elongation are indicators of the ductility of a material. All of these values are located in Table 4. A more ductile material will have a greater percent elongation, and the material will neck down further, resulting in a greater reduction of area. The A36 steel samples had the greatest reduction of area due to the large amount of necking just before fracture. The polycarbonate had the highest percent elongation due to the straightening of the polymer chains. The polymer chains did not neck down after they were straightened, which resulted in a smaller percent reduction of area compared to the steel and aluminum samples. The aluminum did not elongate as far as the steel due to the alloying of the material and the precipitation hardening that was used to improve other properties. The PMMA had the lowest percent reduction of area and the lowest percent elongation, indicating that it is a brittle material. The true stress and true strain take into account the changing area of the cross section as it is being elongated, and the strains that accompany the changing area. Accounting for these two effects results in a final true stress that is much higher than the engineering fracture stress and a greater amount of strain. As shown in Figure 7, the true stress reaches a maximum at the point of fracture. At this point, the area is much smaller, so the specimen cannot withstand a large load, which causes the engineering stressstrain curve to drop off after necking. There is no ultimate tensile stress in the true stressstrain curve 13
14 as with the engineering stressstrain curve, and the true stress is always increasing up until fracture. The RambergOsgood model proved to be excellent at determining the true stress at higher values of true plastic strain, but had higher error at low values of true plastic strain, especially near the yield strain, where plastic strain is essentially zero. Table 5 shows that near the ultimate tensile strain, the error is very small, but near the yield strain, the error is rather high at 19.84%. The aluminum samples did not exhibit the power hardening behavior that is typical of the RambergOsgood model. The engineering stressstrain curve was flat after yielding, and not curved like the model shows in Figure 8. Since the model was fitted to the data between three times the yield strain, and the ultimate tensile strain, it does not fit the sample well at low values of true plastic strain. This error could be alleviated by fitting multiple models to the curve, or by choosing a different model that better fits the shape of the engineering stressstrain curve. 14
15 Appendix A: Calculating the Engineering Stress and Strain Each material was tested three times, and the Engineering stress was plotted against the engineering strain. To calculate the engineering stress and strain, the Instron machine used extensometers up until necking, which measured the strain induced on the sample. Past necking, the Instron machine obtained strain data from the position of the crosshead. The load cell on the moving crosshead measured the vertical load applied to the sample. The diameter of the gage on the sample was measured using calipers, and from there the area was calculated using Equation A.1. The engineering stress is a function of the force applied and the original crosssectional area of the gage of the sample. Using Equation A.2, the engineering stress was calculated. P denotes the tensile force applied to the specimen. (Equation A.1) (Equation A.2) Appendix B: Determining the Modulus of Elasticity and the Yield Stress The modulus of elasticity and the yield stress was calculated for all three samples of both the aluminum and the steel. To find the modulus of elasticity, a small portion of the stressstrain curve was plotted to only include the linear region around zero strain. The slope of the graph at this point is the modulus of elasticity for that material. Excel was used to plot this portion of the stressstrain curve, and a trend line was added to best fit the data. Using the modulus of elasticity, the yield stress was also found. A line was plotted with the modulus of elasticity as the slope, but it was offset mm/mm of strain. The value of the stress where the two lines cross is the corresponding yield stress. This method is the standard 0.2% offset method used to find the yield stress. The average of each value was calculated, along with the standard deviation, using Equation B.1 and Equation B.2, respectively. (Equation B.1) (Equation B.2) 15
16 The ultimate tensile strength was found by determining the maximum load, and using Equation A.2 to solve for the maximum engineering stress encountered. The standard deviation was also calculated for the ultimate tensile strength, using Equation B.2. Appendix C: Determining the Modulus of Resilience and the Modulus of Toughness The modulus of resilience is defined as the area under the engineering stressstrain curve up until yielding. It is the maximum energy per unit volume that the sample can absorb elastically. This energy can be recovered by relaxing the stress. Both Equation C.1 and Equation C.2 can be used to calculate the modulus of resilience. (Equation C.1) (Equation C.2) The modulus of toughness is defined as the area under the entire stressstrain curve up until fracture. It is the maximum energy per unit volume that the sample can absorb before it fails completely due to fracture. Unlike the modulus of resilience, most of the energy cannot be recovered by relaxing the stress. The plastic deformation of the material is permanent. The modulus of toughness cannot be calculated using an equation due to the variety of shapes encountered in the stressstrain curves. To find the modulus of toughness for the four materials, one of the three samples was chosen from each material (All of the data was taken from Sample 1 of each material). The data was loaded into MATLAB using XLSREAD, and the area under the curve was evaluated using the TRAPZ command. The cumulative integral from zero strain up until the fracture strain was recorded as the modulus of toughness. The modulus of resilience was also calculated using MATLAB, but the integral was only carried out to the value of the yield strain. 16
17 Appendix D: Determining the True Fracture Strength, Percent Reduction in Area, and Percent Elongation The true fracture strength provides the actual stress at fracture. The engineering stress does not account for the reduction in area due to necking. Equation D.1 provides the true stress at fracture. The diameter of the gage of the specimen was measured after fracture using calipers, and the area of the cross section was calculated using equation A.1. represent the load and the area at fracture, respectively. and (Equation D.1) The percent reduction in area and the percent elongation provide useful information about the ductility of the material. A more ductile material typically has a higher percent elongation up until fracture, and the reduction in area is greater as the material necks down before fracture. A brittle material will not elongate much past the yield strain, and the percent reduction of area is lower than for a ductile material. Equation D.2 is used to calculate the percent reduction in area. is the area at fracture, and is the area of the cross section before testing, both taken from caliper measurements before and after the tensile test. ( ) (Equation D.2) Equation D.3 is used to calculate the true length of the specimen just before fracture. The length measured after fracture is less than the length before due to the elastic recovery when the stress is relieved when the material fractures. is the length of the gage post fracture, and is the engineering stress at fracture. The length after fracture was measured by placing the two halves of the specimen back together, and measuring the length of the gage. Equation D.4 is then used to calculate the percent elongation of the material. (Equation D.3) ( ) (Equation D.4) 17
18 Appendix E: Determining the True Stress and the True Strain The true stress and true strain was calculated for one sample of aluminum, in this case for the second sample. The engineering stress and strain does not account for the reduction in area as the sample is pulled apart, nor does it account for strains besides the axial direction. The true stress and true strain show the actual stress and strain encountered during the tensile test. The true stress can be calculated at any point using Equation E.1, but since the instantaneous area was not known for this test, other methods had to be incorporated. denotes the true stress. The tensile force is denoted by P, and the instantaneous area is shown by A. (Equation E.1) For strains below two times the yield strain, the true stress is well approximated by the engineering stress, shown by Equation E.2. Between two times the yield strain and necking (the strain at the ultimate tensile stress), the true stress is approximated by Equation E.3. is the engineering stress, and is the engineering strain. (Equation E.2) (Equation E.3) The true strain was calculated using Equation E.4, up until necking. From necking until fracture, there was not enough information to fully define the true stress or true strain. The final true stress was calculated using the final area and the tensile force right before fracture, as shown in Equation E.5. The true strain at fracture was calculated using Equation E.6. A final point was plotted, and a straight line was drawn from necking to fracture. is the tensile force at fracture. (Equation E.4) (Equation E.5) ( ) (Equation E.6) 18
19 Log(True Stress) Appendix F: The RambergOsgood Equation for Plastic Deformation After the true stress and true strain were calculated, the true plastic strain was calculated using Equation F.1. This resulted in the elastic strain being taken out, leaving only the permanent plastic strain. The true elastic strain was calculated using Equation F.2. (Equation F.1) (Equation F.2) A plot was made of the logarithm of the true stress versus the logarithm of the true plastic strain. The plot only concerned the region between three times the yield strain, and the strain corresponding to the ultimate tensile stress. This resulted in a straight line that was fit with a best fit model of the curve, yielding a linear equation, as shown in Figure F.1. y = x Log(True Plastic Strain) 2.58 Figure F.1: The plot of the logarithm of the true stress versus the logarithm of the true plastic strain Excel was used to create the linear equation, and the slope and y intercept were used to create a model of the true stress encountered, using the true plastic strain, according to Equation F.3. (Equation F.3) 19
20 Using logarithm identities, the slope of the equation ( ) became n in Equation F.3, and 10 raised to the power of the y intercept (2.6909) became H (490.8) in Equation F.3. The resulting equation is shown as Equation F.4. (Equation F.4) Equation F.4 was used to create a plot of the true stress versus the true strain to compare it to the experimental plot of the true stress versus the true strain, as shown in Figure 8. The equation was also used to calculate the true stress at set values of true plastic strain of 0.001, 0.01, and The calculated values of the true stress were compared to the true stress values obtained from the experiment in Table 5 using percent error. 20
Objectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationMAE 20 Winter 2011 Assignment 5
MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the
More informationAdam Zaborski handouts for Afghans
Tensile test Adam Zaborski handouts for Afghans Outline Tensile test purpose Universal testing machines and test specimens Stressstrain diagram Mild steel : proportional stage, elastic limit, yielding
More informationTensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationTensile Testing of Steel
C 265 Lab No. 2: Tensile Testing of Steel See web for typical report format including: TITL PAG, ABSTRACT, TABL OF CONTNTS, LIST OF TABL, LIST OF FIGURS 1.0  INTRODUCTION See General Lab Report Format
More informationPLASTIC DEFORMATION AND STRESSSTRAIN CURVES
PLASTIC DEFORMATION AND STRESSSTRAIN CURVES Introduction Background Unit: Plastic Deformation and StressStrain Curves In the last unit we studied the elastic response of materials to externally applied
More informationUniaxial Tension and Compression Testing of Materials. Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng
Uniaxial Tension and Compression Testing of Materials Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng 3.032 Lab Report September 25, 2013 I. Introduction Understanding material mechanics
More informationStress Strain Relationships
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationME 215 Engineering Materials I
ME 215 Engineering Materials I Chapter 3 Properties in Tension and Compression (Part III) Mechanical Engineering University of Gaziantep Dr. A. Tolga Bozdana www.gantep.edu.tr/~bozdana True Stress and
More informationSTRAINLIFE (e N) APPROACH
CYCLIC DEFORMATION & STRAINLIFE (e N) APPROACH MONOTONIC TENSION TEST AND STRESSSTRAIN BEHAVIOR STRAINCONTROLLED TEST METHODS CYCLIC DEFORMATION AND STRESSSTRAIN BEHAVIOR STRAINBASED APPROACH TO
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationStructures and Stiffness
Structures and Stiffness ENGR 10 Introduction to Engineering Ken Youssefi/Thalia Anagnos Engineering 10, SJSU 1 Wind Turbine Structure The Goal The support structure should be optimized for weight and
More informationMechanical Properties
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationUnit 2: Science for Engineering LO4: Understand properties of materials  Forceextension graphs Instructions and answers for teachers
Unit 2: Science for Engineering LO4: Understand properties of materials  Forceextension graphs Instructions and answers for teachers These instructions should accompany the OCR resource Forceextension
More informationPlastic Behaviour  Tensile Strength
Plastic Behaviour  Tensile Strength Transition of mechanical behaviour from elastic to plastic depends upon the material type and its condition as tested (hotrolled, coldrolled, heat treated, etc.).
More informationTENSILE TESTING PRACTICAL
TENSILE TESTING PRACTICAL MTK 2B Science Of Materials Ts epo Mputsoe 215024596 Summary Material have different properties all varying form mechanical to chemical properties. Taking special interest in
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationσ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More informationMechanics of MaterialsSteel
Mechanics of MaterialsSteel Structural Steel Structural steel considered one of the predominant materials for construction of buildings, bridges, towers and other structures. The preferable physical properties
More informationPROPERTIES OF MATERIALS
1 PROPERTIES OF MATERIALS 1.1 PROPERTIES OF MATERIALS Different materials possess different properties in varying degree and therefore behave in different ways under given conditions. These properties
More informationSolution for Homework #1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
More informationProblem P5.2: A 1 Mg container hangs from a 15 mm diameter steel cable. What is the stress in the cable?
Problem P5.: A 1 Mg container hangs from a 15 mm diameter steel cable. What is the stress in the cable? Find the cross sectional area in terms of diameter using Equation (5.1). Calculate the tensile stress
More informationMUKAVEMET KIRILMA HİPOTEZLERİ
1 MUKAVEMET KIRILMA HİPOTEZLERİ 17. Theories of failure or yield criteria (1) Maximum shearing stress theory (2) Octahedral shearing stress theory (3) Maximum normal stress theory for brittle materials.
More informationStandard Test Procedures Manual
STP 20319 Standard Test Procedures Manual Section: 1. SCOPE 1.1. Description of Test The Force Ductility test is a measure of the tensile properties of the polymer modified asphalt cement residue of a
More informationProperties of Materials
CHAPTER 1 Properties of Materials INTRODUCTION Materials are the driving force behind the technological revolutions and are the key ingredients for manufacturing. Materials are everywhere around us, and
More informationσ y ( ε f, σ f ) ( ε f
Typical stressstrain curves for mild steel and aluminum alloy from tensile tests L L( 1 + ε) A =  A u u 0 1 E l mild steel fracture u ( ε f, f ) ( ε f, f ) ε 0 ε 0.2 = 0.002 aluminum alloy fracture
More informationCitation Journal of Constructional Steel Research, 2014, v. 96, p
Title The Art of Coupon Tests Author(s) Huang, Y; Young, B Citation Journal of Constructional Steel Research, 014, v. 96, p. 159175 Issued Date 014 URL http://hdl.handle.net/107/00516 Rights NOTICE: this
More informationProperties of Matter
Mr. Patrick J Camilleri B.Ed (Hons) M.Ed Science (Sheffield) Department of Physics JC Malta Properties of Matter Basics You Should Know Elasticity. Young modulus 1. Hooke's law. Extension α tension (force
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationMaterial Testing Lab
Focus: Material Testing Lab This laboratory includes three separate materials testing experiments to be done on spaghetti of 3 different diameters. See individual labs for respective objectives. Students
More informationMCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions
MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions The Quiz questions based upon HW9 will open on Thursday, Apr. 11 and close on Wednesday, Apr 17 at 1:30 PM. References to A&J: Chapters 13,
More informationInteraction of Hydrogen and Deformation in 316L Stainless Steel
Proceedings of the SEM Annual Conference June 14, 2009 Albuquerque New Mexico USA 2009 Society for Experimental Mechanics Inc. Interaction of Hydrogen and Deformation in 316L Stainless Steel Bonnie R.
More informationMAE 20 Winter 2011 Assignment 6
MAE 0 Winter 011 Assignment 6 8.3 If the specific surface energy for sodalime glass is 0.30 J/m, using data contained in Table 1.5, compute the critical stress required for the propagation of a surface
More informationCHAPTER 4 TENSILE TESTING
CHAPTER 4 TENSILE TESTING EXERCISE 28, Page 7 1. What is a tensile test? Make a sketch of a typical load/extension graph for a mild steel specimen to the point of fracture and mark on the sketch the following:
More informationTorsion Testing. Objectives
Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials
More informationGriffith theory of brittle fracture:
Griffith theory of brittle fracture: Observed fracture strength is always lower than theoretical cohesive strength. Griffith explained that the discrepancy is due to the inherent defects in brittle materials
More informationUniversity of Portland School of Engineering LABORATORY OUTLINE: TENSILE TESTING OF STEEL & ALUMINUM ALLOYS (ASTM E8)
TENSILE TESTING OF STEEL & ALUMINUM ALLOYS (ASTM E8) To carry out a standard tensile test on specimens of a hot rolled steel (AISI 1045), Type 2024 T351 aluminum, polymers (UHMWPE, acrylic) and, from
More informationUROP Annealed 3D printed parts Final Write up Michael Rosplock Abstract
UROP Annealed 3D printed parts Final Write up Michael Rosplock Abstract The purpose of this study was to examine the effects of a basic annealing process on 3D printed tensile test samples. Several different
More informationCH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More informationFAILURE MODES and MATERIALS PROPERTIES. Component failures. Ductile and Brittle Fracture COMPONENT FAILURES. COMPONENT FAILURE MODES examples:
FAILURE MODES and MATERIALS PROPERTIES MECH2300  Materials Lecture 10 R. W. Truss Materials Engineering R.Truss@uq.edu.au COMPONENT FAILURES Structures lectures es on component es cause response in component
More informationFatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY)
Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY) Ali Fatemi, Jonathan Williams and Farzin Montazersadgh Professor and Graduate
More informationDescription of mechanical properties
ArcelorMittal Europe Flat Products Description of mechanical properties Introduction Mechanical properties are governed by the basic concepts of elasticity, plasticity and toughness. Elasticity is the
More informationMECHANICS OF SOLIDS COMPRESSION MEMBERS TUTORIAL 1 STRUTS. On completion of this tutorial you should be able to do the following.
MECHANICS OF SOLIDS COMPRESSION MEMBERS TUTORIAL 1 STRUTS You should judge your progress by completing the self assessment exercises. On completion of this tutorial you should be able to do the following.
More informationMIME 3330 Mechanics Laboratory LAB 5: ROTATING BENDING FATIGUE
MIME 3330 Mechanics Laboratory LAB 5: ROTATING BENDING FATIGUE Introduction In this experiment, the finite life fatigue behavior of a smooth cylindrical specimen as shown in Figure 1 will be studied in
More informationREINFORCED CONCRETE. Reinforced Concrete Design. A Fundamental Approach  Fifth Edition
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition CONCRETE Fifth Edition A. J. Clark School of Engineering Department of Civil and Environmental Engineering
More informationMENG 302L Lab 4: Modulus of Elasticity and Poisson s Ratio
MENG 302L Lab 4: Modulus of Elasticity and Poisson s Ratio Introduction: In Lab 4 we will measure the two fundamental elastic constants relating stress to strain: Modulus of Elasticity and Poisson s Ratio.
More informationPhysics 3 Summer 1989 Lab 7  Elasticity
Physics 3 Summer 1989 Lab 7  Elasticity Theory All materials deform to some extent when subjected to a stress (a force per unit area). Elastic materials have internal forces which restore the size and
More informationEffect of Heat Treatment Processes on the Mechanical Properties of Medium Carbon Steel
Journal of Minerals & Materials Characterization & Engineering, Vol. 11, No.2 pp.143152, 2012 jmmce.org Printed in the USA. All rights reserved Effect of Heat Treatment Processes on the Mechanical Properties
More informationSolid Mechanics. Stress. What you ll learn: Motivation
Solid Mechanics Stress What you ll learn: What is stress? Why stress is important? What are normal and shear stresses? What is strain? Hooke s law (relationship between stress and strain) Stress strain
More informationLong term performance of polymers
1.0 Introduction Long term performance of polymers Polymer materials exhibit time dependent behavior. The stress and strain induced when a load is applied are a function of time. In the most general form
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME 2 ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
More informationM n = (DP)m = (25,000)(104.14 g/mol) = 2.60! 10 6 g/mol
14.4 (a) Compute the repeat unit molecular weight of polystyrene. (b) Compute the numberaverage molecular weight for a polystyrene for which the degree of polymerization is 25,000. (a) The repeat unit
More informationdifferent levels, also called repeated, alternating, or fluctuating stresses.
Fatigue and Dynamic Loading 1 Fti Fatigue fil failure: 2 Static ti conditions : loads are applied gradually, to give sufficient i time for the strain to fully develop. Variable conditions : stresses vary
More informationPOWER SCREWS (ACME THREAD) DESIGN
POWER SCREWS (ACME THREAD) DESIGN There are at least three types of power screw threads: the square thread, the Acme thread, and the buttress thread. Of these, the square and buttress threads are the most
More informationObjective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels.
IMPACT TESTING Objective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels. Equipment Coolants Standard Charpy VNotched Test specimens Impact tester
More informationSheet metal operations  Bending and related processes
Sheet metal operations  Bending and related processes R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Table of Contents 1.QuizKey... Error! Bookmark not defined. 1.Bending
More informationMaterial Science Engineering and Steel Making/Metallurgy. Stark County High Schools 2016
Material Science Engineering and Steel Making/Metallurgy Stark County High Schools 2016 Agenda What is Material Science Engineering Basics of Steel Making Steel Processing and Properties 2 What is Material
More informationImpact testing ACTIVITY BRIEF
ACTIVITY BRIEF Impact testing The science at work Impact testing is of enormous importance. A collision between two objects can often result in damage to one or both of them. The damage might be a scratch,
More informationPHYSICAL TEST OF STAINLESS STEEL 316 BETWEEN DIFFERENT MANUFACTURES
PHYSICAL TEST OF STAINLESS STEEL 316 BETWEEN DIFFERENT MANUFACTURES ZAITUL AQMAR BT MOHD ASRI Thesis submitted in partial fulfilment of the requirements for the award of the degree of Bachelor of Chemical
More informationSHORE A DUROMETER AND ENGINEERING PROPERTIES
SHORE A DUROMETER AND ENGINEERING PROPERTIES Written by D.L. Hertz, Jr. and A.C. Farinella Presented at the Fall Technical Meeting of The New York Rubber Group Thursday, September 4, 1998 by D.L. Hertz,
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationConcepts of Stress and Strain
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original
More informationEffect of Temperature and Aging Time on 2024 Aluminum Behavior
Proceedings of the XIth International Congress and Exposition June 25, 2008 Orlando, Florida USA 2008 Society for Experimental Mechanics Inc. Effect of Temperature and Aging Time on 2024 Aluminum Behavior
More informationMaterial property tests of Smoothon Vytaflex60 liquid rubber
Material property tests of Smoothon Vytaflex60 liquid rubber Sanjay R. Arwade March 16, 2006 During the fall semester of the 20052006 academic year, I decided to try to produce some scale models of structural
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
14:440:407 Fall 010 Additional problems and SOLUTION OF HOMEWORK 07 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 To provide
More informationFatigue Failure Due to Variable Loading
Fatigue Failure Due to Variable Loading Daniel Hendrickson Department of Computer Science, Physics, and Engineering University of Michigan Flint Advisor: Olanrewaju Aluko 1. Abstract Fatigue failure in
More informationME 612 Metal Forming and Theory of Plasticity. 3. Work Hardening Models
Metal Forming and Theory of Plasticity Yrd.Doç. e mail: azsenalp@gyte.edu.tr Makine Mühendisliği Bölümü Gebze Yüksek Teknoloji Enstitüsü In this section work hardening models that are applicable to different
More informationAN EXPLANATION OF JOINT DIAGRAMS
AN EXPLANATION OF JOINT DIAGRAMS When bolted joints are subjected to external tensile loads, what forces and elastic deformation really exist? The majority of engineers in both the fastener manufacturing
More informationMechanical properties 3 Bend test and hardness test of materials
MME131: Lecture 15 Mechanical properties 3 Bend test and hardness test of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Bend test of brittle materials Hardness testing
More informationFigure 1: Typical SN Curves
StressLife Diagram (SN Diagram) The basis of the StressLife method is the Wohler SN diagram, shown schematically for two materials in Figure 1. The SN diagram plots nominal stress amplitude S versus
More informationIntroduction to Tensile Testing
CHAPTER 1 Introduction to Tensile Testing TENSILE TESTS are performed for several reasons. The results of tensile tests are used in selecting materials for engineering applications. Tensile properties
More informationChapter 12 Elasticity
If I have seen further than other men, it is because I stood on the shoulders of giants. Isaac Newton 12.1 The Atomic Nature of Elasticity Elasticity is that property of a body by which it experiences
More informationDistinguishing strength from toughness. Understanding fracture toughness.
Lecture notes version 20 Oct 2010 Chapter 8 Fracture and fracture toughness A fractured Liberty Ship 8.1 Introduction and synopsis Distinguishing strength from toughness. Understanding fracture toughness.
More informationSTRESSSTRAIN CURVES
STRESSSTRAIN CURVES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 August 23, 2001 Introduction Stressstrain curves are an extremely
More informationExperiment: Mechanical Testing Impact & Hardness Testing
Experiment: Mechanical Testing Impact & Hardness Testing Objective The main objective of this experiment is to introduce two important basic mechanical property tests; hardness (using Rockwell testing)
More informationBME 315 Biomechanics Material Properties of Tendon: introduction
: introduction Adapted by R. Lakes from D. Thelen and C. Decker, U. Wisconsin, 09 I. Introduction In this lab, we will investigate the material properties of a tendon. Tendons and ligaments are very similar
More informationEffects of Sulfur Level and Anisotropy of Sulfide Inclusions on Tensile, Impact, and Fatigue Properties of SAE 4140 Steel
Paper 281434 Effects of Sulfur Level and Anisotropy of Sulfide Inclusions on Tensile, Impact, and Fatigue Properties of SAE 414 Steel Copyright 28 SAE International Nisha Cyril and Ali Fatemi The University
More informationComparison of typical 3D printing materials [1]
Comparison of typical 3D printing materials [1] ABS Its strength, flexibility, machinability, and higher temperature resistance make it often a preferred plastic for engineers, and professional applications.
More informationTEST REPORT. Rendered to: LMTMercer Group, Inc. For: PRODUCT: 4" x 4" and 5" x 5" PVC Porch Posts with Aluminum Reinforcing
TEST REPORT Rendered to: LMTMercer Group, Inc. For: PRODUCT: 4" x 4" and 5" x 5" PVC Porch Posts with Aluminum Reinforcing Report No.: Report Date: 01/28/14 Test Record Retention Date: 12/20/17 130 Derry
More informationStress Strain Behavior (I) Stress Strain Behavior (II) Stress Strain Behavior (III)
Chapter Outline: Characteristics, Applications, and Processing of Polymers Mechanical properties StressStrain Behavior Deformation of Semicrystalline Polymers Crystallization, Melting, Glass Transition
More informationHardness Testing. Objectives
Laboratory 2 Hardness Testing Objectives Students are required to understand the principles of hardness testing, i.e., Rockwell, Brinell and Vickers hardness tests. Students are able to explain variations
More information15. MODULUS OF ELASTICITY
Chapter 5 Modulus of Elasticity 5. MODULUS OF ELASTICITY The modulus of elasticity (= Young s modulus) E is a material property, that describes its stiffness and is therefore one of the most important
More informationValidation of Cable Bolt Support Design in Weak Rock Using SMART Instruments and Phase 2
Validation of Cable Bolt Support Design in Weak Rock Using SMART Instruments and Phase 2 W.F. Bawden, Chair Lassonde Mineral Engineering Program, U. of Toronto, Canada J.D. Tod, Senior Engineer, Mine Design
More informationTeaching Graphical Data Presentation Techniques in an Introductory Materials Course
Indiana University  Purdue University Fort Wayne Opus: Research & Creativity at IPFW Manufacturing and Construction Engineering Technology Faculty Publications Department of Manufacturing and Construction
More informationNOTCHES AND THEIR EFFECTS. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1
NOTCHES AND THEIR EFFECTS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations SN Approach for Notched Members
More informationEffect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel
International International Journal of ISSI, Journal Vol. of 12 ISSI, (2015), Vol.10 No.1, (2013), pp. 2832 No.1 Effect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel M. Mehdinia
More informationTable 1 Typical Physical and Thermal Properties of Mylar Polyester Film. Property Typical Value Unit Test Method
Product Information Mylar polyester film PhysicalThermal Properties Mylar polyester film retains good physical properties over a wide temperature range ( 7 to 15 C [ 9 to 3 F]), and it is also used at
More informationMODULUS ELASTICITY REPORT
MODULUS OF ELASTICITY REPORT September 24 th, 2003 Report Prepared By: Sean Mulligan Testing Performed By: Bob Thompson Chuck Cook Donita Weatherspoon Modulus of Elasticity Report PURPOSE The purpose of
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationDESIGN AND DEVELOPMENT OF AN ECONOMICAL TORSION TESTING MACHINE
DESIGN AND DEVELOPMENT OF AN ECONOMICAL TORSION TESTING MACHINE by GLENN E. VALLEE ASSISTANT PROFESSOR MECHANICAL ENGINEERING and ROBERT SHORT WESTERN NEW ENGLAND COLLEGE SPRINGFIELD MASSACHUSSETS Session
More informationApplication of WebBased Bar Fatigue Database. Database Development
Application of WebBased Bar Fatigue Database Database Development Thomas G. Oakwood Bar Steel Fatigue Database Objectives Develop a straincontrolled fatigue database for carbon and low alloy bar steels
More informationStress Relaxation Study of Paper and Plastic Film based Packaging Material
Master's Degree Thesis ISRN: BTHAMTEX2009/D02SE Stress Relaxation Study of Paper and Plastic Film based Packaging Material Rajdip Roy Lu Qi Department of Mechanical Engineering Blekinge Institute
More informationMechanical joining Tensile shear testing of single joint specimens Specimen dimensions and test procedure
Mechanical joining Tensile shear testing of single joint specimens Specimen dimensions and test procedure Assemblage mécanique Essais quasi statiques de tractioncisaillement des échantillons à jonction
More informationHardened Concrete. Lecture No. 14
Hardened Concrete Lecture No. 14 Strength of Concrete Strength of concrete is commonly considered its most valuable property, although in many practical cases, other characteristics, such as durability
More informationStress. tensile. elongation at yield. yield stress. weight. elascity modulus. strain velocity 13%/min
3 Mechanical Properties 3 1 Tensile Strength The strain curve when tension is applied to ASTMD638 type 1 test piece of Iupilon / NOVAREX at a strain velocity of 5mm/min is shown in Fig. 3 1 1. The following
More information